# Fatigue Criteria for Ship Structure Details

Save this PDF as:

Size: px
Start display at page:

## Transcription

1 THE SOCIETY OF NAVAL ARCHITECTS AND MARINE ENGINEERS >e One World Trade Center, Suite 1369, New York, N,Y, >? *3 PaPer\$ to be presented at Extreme load. R,SPO S, ~ : Arli ston, VA, October 19-20, 1981 Symposium ;+ co. 5 %,*L.,*,,+\ Fatigue Criteria for Ship Structure Details W. H. Munse, University of Illinois, U;bana, IL ABSTWCT Fatigue criteria are presented for the design of ship structures. l%e criteria take into account the ship s tructure details, the fatigue resistance of specific locations in these details, the variable loading to which a ship is subj ected, and the desired level of reliability (factor of safety) A design example indicates the simple manner in which the criteria can be useti. NOMENCLATURE log c fs(s) The life intercept of the S-N curve Probability density function- Weibull distribution (Equation 2) (s~ax)n = The maximum stress range of a variable Ioadi g history that is expec ed to produce failure in 10~ cycles N Io8 w L r us = Mean constant-cycle stress range for failure at N cycles. = The maximum stress range expected to occur once in 108 cycles, based o a Weibull distribution. = Characteristic value of S (Equation 5) = Scatter factor (Equation 11) = Gamma func tio = Mean stress of the Weibull distribution (Equation 3) k Shape parameter for the Weibull distribution E = Random load factor (Equation ) L(n) m N (PF) F s SD (sd)all = The probability of m failure through a life, n (Equation 9) Negative slope of S-N curve The mean life necessary to produce a useful life n with a reliability of L(n) Probability = [l-l(n)] of failure Reliability factor (Equation 13) Stress range Constant-cycle fatigue design stress range for a useful life n and reliability L(n) The maximum allowable fatigue stress range (Equation 15) 5s N INTRODUCTION = Standard ieviation of the Weibull distribution. = Total uncertainty in fatigue life (coefficient of variation) Fatigue cracking in ships has been a serious problem for many years As noted by Vedeler (1)1 in 1962, shipbuilders in Norway and Sweden cons idered the problem of fatigue in ships to be of more practical importance for ordinary ships than the question of brittle fracture, He noted that fatigue cracks were often found in the forepeak region, bottom amidships, at the bulwark at both ends of the bridge, and in the hatch corners In a recent stuciy it has been observed that ships may also have cracks at crossings of frames, longitudinal, and girders, and many other locations (2, 3 and 4) in 1 Reference parentheses. numbers are indicated & 23.1

2 Since such cracks may be possible points of initiation for catastrophic failures and, since the repair of fatigue cracks can be very costly, it is essential that fatigue be given adequate consideration i the design of ship structures In this paper criteria are pz-esented for the fatigue design of ship structural details along with a brief discussion of the principal parameters included in the criteria. 2 An example of the application of these design crireria is then presented to indicate the simple manner in which the criteria can be used to provide a verification of the adequacy of a ship in fatigue. FATIGUE DESIGN PARAMETERS Fatigue design generally consists of verifying that the details of a structure have sufficient resistance to repeated loading to provide a fatigue life equal to or greater than required: a wrifica, tion by checking Drocess To achieve this for shiu ;tructure details, criteria have ~een de eloped which takes into account, (a) the basic fatigue behavior of welded structural details, (b) the types Of details found in ship structures at which cracking has been observed, (c) the loading histories to which ships may be subjected, and (d) the level of fatigue safety to be included in the ship design. There are other factors that can affect the fatigue behavior of a structure also ; however, their importance or effect is not as great as the effect o f those noted above and to include them would have greatly complicated the overall design process. These neglected factors include, (a) the mean stress effect, an effect that is relatively small for welded details and is now neglected in most fatigue design specifications, (b) the tensile strength of the steel, another factor that is generally neglected in structural fatigue design specifications and considered to have relatively little effect in long life fatieue. and (c) tempera ture,-rate of lo~d application, residual stresses, and size effect, again factors that are Eenerally found to be of secondary Zmport anie Fatigue Behavior of Weldments During the nearly 50 years of laboratory studies conducted on weldments, numerous papers, conference proceedings and books have been published wherein detailed fatigue data for welds and weldments may be found (5-11) Recently, much of this information has been re-examined to estab. lish basic S-N relationships for numerous types of welded members and details (12) Nearlv 1500 S-N curves have beeri p;oduced, &ne example of which is presented in Fig. 1. (This is the S-N curve for axially loaded longitudinal fdl penetration groove welds with the reinforcement intact; based on stress range; and for mild, high strength low alloy or quenched and tempered steels. Identified by DAAAXB) The solid line mean regression curve (50% reliability) of Fig. 1, as established by a least-square analysis, can be given by, Log N=log C-mlog SN (1) where, log c = N= m= ~; or SN = (N) (la) the life intercept of the S-N curve number of cycles to failure for a constant cycle stress range of SN, the negatiw slope of the S-N curve N = the constant-cycle stress range for failure at N cyci es. Using such straight-line relationships, the mean fati ue stress ranges for lives of 105, 10~, 10, 108 cycles, have been established for numerous welded members and details, and are presented in Table 13, These mean fatigue strengths are for the numerous structural fatigue details shown in Fig. 2. For each of the details shown in Fig. 2, the location at hich the fatigue strength applies is the point where the greatest *tress concentration exists and, except as noted, ca be 2 The ship design criteria presented herein were developed in an investigation conducted at the University of Illinois and sponsored by tbe Snip Structure Committee, 3 Under random loadings straightline S-N relationships are found to extend well beyond the fatigue limits often reported for constant cycle tests (10) Therefore: in this development, the straight-line S-N relationship has been assumed to extend to 108 cycles or more. 232

3 I ! Ill [ ) [ Iu J 1 1 1, 1 I ++~ LB,,? TGLFFCNU L,!, s,,. 5..,, K (OJ 9,,: CO.r)[)[kct LCWL - m 60. m.,,. = =- -- =--- t _ thth }+ H, 5, 10,!, :,, 5,,,, CYCLES TO FF!lLL!RE,IN TH12U5RNC 5 Fig. 1. S-N Relationship for a Weldment Containing a Longitudinal Groove weld in the As-Welded Condition, (Detail No. 3) considered to be a function of the principal tensile stress at that location. This location, for example, is at the end of the cover plate for detail No. 5, is at the toe of the butt weld for detail No. 10, and is at the side of the hole in detail No. 28. The data in Table I and the diagrams of Fig. 2 provide the basic fatigue information on which the fatigue design criteria presented herein are based. been identified and will provide guidance in locating the details for which possible fatigue failure should be checked (22) AII example of a few of these families and configurations of details is presented in Fig. 3. The locations in Fig. 3 at which fatigue cracking might develop are circled and identified by the correspond- ~g structural detail number from Fig, (The basic fatizue resistance for the detail is provi~ed in Table 1) Ship Details After the basic fatigue data had been assenbled, the second phase in the development of tbe fatigue design procedure was the identification of those ship locations at which fatigue crackine mi zht occur. Two recent reports o; th~ in-service performance of structural ship details (3, 4) have served to define possible fatigue criti - cal locations in &hips These-reports catalog and define the types and locations of details at which failures have occured in a variety of merchant and Naval vessels. A total of 86 ships were included in the surveys The details examined were separated into twelve general families (see Table II) and these were in turn divided into 56 zrouds of 634 separate configurations. - A ~otal of 6856 failures were found in the details observed. In the investigation on which this paper is based, the locations in each of these confi~urations at which fatigue might devel~p have Not all details in Fig, 2 are found in ships and not all of the details used in the ships surveyed ha e exhibited cracks Only the thirty-seven details listed in Table III are those for which cracking was reported and then, some of the details exhibited only a very limited number of cracks Those for which the largest number of cracks were found are those for which these fstigue design criteria will be of svceatest value, However. in design a?atig e evalwition shodd be made-of all details for which fatigue cracking is a possibility, Ship Loadings To properly evaluate the fatigue adequacy of a ship detail requires a realistic estimate of the cvclic stress history to which the detail-will be subjected during its lifetime. Since the existing full-scale ship loading data are for a limited length of time. it has been necessary to-extrapolate the available data to obtain an estimated lifetime spectrum (13, 14) Such 233

4 TASLE I Mean Fatigue Stress Range for Fatigue Details in Fig. 2 (Constant Cycle - 0,50 Reliability) Detalil S-N Stress Range, ksi, for n cycles2 Slope, (seyijig, 2) m ~ = 105 ~ = 106 = 10 ~ = (F) (G) , , , , ,0 29, , , , , , (s) 10 1O(G) 11 11(G) 12(G) :! (G) 1(s) , ,8 55, ,8 35, ,6 25,98 32, ,8 28, ,2 25, 3 29, , , ,6 15, , , , ,91 12, , , (s) 19 19(s) 20 20(s) 21 21(s) A 25B , , (:;;:) 39, (;::;) ,00 20,28 18, (~M:36) 19, ,1 (;:::;) 14, (;;:;3) 9,22 8,68 8, (M:j:) , , (5,0) ,43 4, (::~:) (S) 28 28(F) 29 ;;#) ,8 40,1 (29.4) (18.21) 8,16 22,11 (11,28) (6,99) 29R2 30 2,83 38~0 16,83,46 3,31 234

5 TABLE I (CONTINUED) Detail S-N Stress Range, ksi, for n cycles2 No.1 Slope, (See Fig. 2) m n = 105 ~ = 106 n=10 ~ = A 31 ;;A 32B 32c ::(s) (::;;) 3; (34.o) (20,16) (;::g:) 21;34 25,5 (23.5) (11.8) (;:i;y) 11~38 20,45 (16.1) (6.99) (:;:;) 6; (:;:;:] (:;:;) 3; (s) A 3 3s (21.34) (:::;) (11.38) (;;:\$:) , (6.0) (1::::) 10, ;24 (3.23) (1::l..) :9 :; (s) , A 39B 39C (21~50) 110,2 (11:21) 69;8 (5;84) 44,08 (3:04) 2; A A 48 4:35 (20~16) (11~8) (6:99) (4112) 48R (S) Indicates shear stress on fasteners or welds (F) Indicates flame cut surfaces. (G) Indicates the surfaces have been ground flush Estimated values are shown in parentheses ( ) A dash is provided where no data are available 235

6 -==2-29( F)-29 29RI (Radi.3 = l14~,to1/2 ) 29 R2(Rodi. s,1/2 Iol ) w. c C===D > 30A 3;(s)-3 ) c 38( S)-38 c e= c 1 3 1,, -, / - L~ # &&J-&. 32 f3==j-yp- 13 Fig. 2, Structural Fatigue - Details 236 _.

7 T (a) Family No.I(AI) T ,21 (b) Family No,l(B4) 42 \ b 25B 2130 Zf(s) (c) Family No, 2 (c2) m W_ 25 ; 33 33s (d) Family No. 3( AI) III f (e) Family No,8 (A3) (f) Family No, II(AIO) Fig. 3. Examples of Configurations in ship family details (3,4) 45A TABLE III Details Exhibiting Failures i Ships n ct&jl, Total Detail No. o. No. Crack Detail & Total No. of Cracks *+ 51 k- -#-- 52 r-l L.. c3cj- 4 F / / 53 (G) - Designates a ground surface (S) - Designates shear on weld or fastener (F) Designates flame-cut edges f.aicomparison with machined edges Fig,2, Structural Fatigue-Details (cent s 19 19s s F 29 29R 29F 30 30A B 33 33s 34 34s R i--

8 ~BLE II Summary of Data for 12 Detail Families (Ref. 4) Totals Observed?amily Detail Family Total No, Total No, z No, Name Details Failures Failures 1 Beam Bracket 68,586 2, B 2 Tripping Bracket 34,o12 1, Non-Tight Collar 20, ,16 4 Tight Collar 20, Gunwale Connect ion Knife Edges o 0 Miscellaneous Cutouts 296, Clearance Cutouts 5, Deck Cutouts, Stanchion Ends, Stiffener Ends 40, Panel Stiffeners 53, ,46 Totals 60,584 6,856 1,13 ) 238